ELSEVIER Thermochimica Acta 298 (1997) 55-58
Impact of zeolitic water content on exchange of calcium ions
P. Sidheswaran*, A.N. Bhat
Hindustan Lever Research Centre, Chakala, Andheri (East), Mumbai 400099, India
Received 6 September 1996; accepted 23 May 1997
4A and P zeolites were thermally treated to dehydrate them to different extents. The residual water content and calcium exchange capacity (CEC) values of the treated zeolites were evaluated. The study revealed that the CEC of the zeolites depended upon the zeolitic water level. Anhydrous zeolites are devoid of exchange capacity. Mixed zeolites demonstrated mineralisation effect and an additional peak in the thermal studies. 1997 Elsevier Science B.V.
Keywords: Zeolites; Calcium; Thermal
1. Introduction are present as hydrated sheaths. Hence, it was felt that the zeolitic pool of water will have a definitive
Zeolites are three-dimensional networks of (Si, A1) role in the exchange capacities. The current investiga- and 04 tetrahedra-linked by sharing of oxygen tion examines the same with Ca 2+ ions as a typical atoms into rings and cages. The overall negative probe. charge of the anion is balanced by cations that are located in the cavities in the network. Zeolites have pore structures with interconnecting channels which 2. Materials and methods are large enough for ions and small molecules such as water to pass freely without disrupting the network 2.1. Materials [ 1,2].Two types of zeolites, namely, 4A [with structure Na12(AIOz)12 (SIO2)12. 27H20] and P [with structure Three different commercial samples of 4A and P Na6(A1Oz)6.(SiO2)6.15H20] have been shown prefer- zeolites were obtained for this study. Two of them ence in the detergent industries for use as builders. The were found to be pure samples (by XRD) and coded as extent of structural water present in the zeolite I and II whereas the third was a mixed zeolite coded as changes with the nature of the zeolite and the III. thermal pre-history of the product. The structural zeolitic water is generally conceived of as a 'pool' 2.2. Methods or 'well' inside the cage. Hardness ions of water
Commercial zeolite samples of 4A and P were dried *Corresponding author: Tel.: 00 91 832 9471 fax: 00 91 022 836 and calcined at different temperatures in the range of
3680 100-900C while monitoring the weight loss. TGA
0040-6031/97/$17.00 1997 Elsevier Science B.V. All rights reserved PII S0040-6031(97)00204-9
56 P Sidheswaran, A.N. Bhat/Thermochimica Acta 298 (1997) 55-58
andDTGAofthesampleswerecarriedouttoobtain ~/~ , J l ,~ [~t ' t 1 ~ ~ i L t / the water content and thermal behaviour.
The samples prepared at different temperatures CSA,PLE ,I~ | . ~ Icl were subjected to XRD studies with a Siemens crystal- ,~_~' ~ '~ uLJW ~;V~ ' ~-~ \-~-W loflex diffractometer using nickel-filtered CuK,~ radia-
tion. Calcium exchange measurements were made by the i l l t ~ / EDTA titration using Eriochrome Black-T as the ~ ~ Vt~j~j ~ indictor . The CEC values were expressed on an
anhydrous basis. J l To quantify the presence of the mixed zeolitic / / phase, synthetic mixtures of 4A/P were prepared I and subjected to XRD studies. The XRD technique was employed to substantiate the role of the miner- c SAMPLE', > alisation effect with mixed zeolites. ~ .~_~ ~f~j ~ t b)
J 3. Result and discussion I /~ IL ]1 ( SAMPLE [ ) ~, I I
3.1. Nature of commercial zeolites __~ ~ ~_ J~ ;~.__ /~ (o,
The XRD patterns of samples of 4A and P are 40 30 20 ~0 presented in Fig. 1. It is clear from Fig. l(a) that 20 ~.cuK.~ P zeolite has characteristic prominent fingerprints Fig. 1. XRD patterns of commercial zeolites:(a) Sample 1-zeolite at 12.4 and 21.8(20) and 4A has prominent P(b) Sample II-zeolite 4A(c) Sample Ill-(mixed zeolite)(d) Blend fingerprints at 7.2, 10.1, 12.4, 21.6, 24.0, 27.0 and of Samples I and II (50:50 w/w) 29.9(20).
It is easy to identify the nature of the zeolitic builder ~oo [~i~ ~ . . . . . . . . . . ~\ - .~ /~ DTGA SAMPLE [ by making a cursory examination of the peaks at 20: ~ ( PURE P)
12.4 and 7.2 and their relative intensities. Some commercial samples contained mixed phases [ J - - - T~A
of zeolites (4A and P). This is demonstrated in ~ ~I, II Fig. l(c). (Fig. l(d) is for 1:1 mixed blend of the zeolites). ~ ~oo -~ ~ j f ~OA
MIXED ZERLITES ( SAMPLE III ) 3.2. Zeolitic water -__ ~
7s i l, i hJ The amount of zeolitic water present is dictated by ,Y the type (nature) of zeolite and the manufacturing
30 210 390 570 750 930 conditions. Thus, for 4A zeolite, the theoretical water content should be 22%. TGA of sample II gave ~21% TEMPERATURE ('C) and the loss on ignition (LOI) studies showed 22%. Fig. 2. TGA and DTGA of pure and mixed zeolite P Hence the match was good.
For P zeolite the LOI ranges between 16.2 to 21.4% normally. This is indeed dictated by the levels of AI are presented in Fig. 2. Similar patterns were noted and Si. Two different P zeolite samples were exam- with pure and mixed zeolite 4A. An examination of ined. One of them showed 19% by TGA as well as LOI Fig. 2 revealed the possibility of identifying mixed studies (Fig. 2).The TGA of pure and mixed zeolite P zeolite phases by this thermal technique.
P.. Sidheswaran, A.N. Bhat/Thermochimica Acta 298 (1997) 55-58 57
3.3. Dehydration 1. Pure 4A and pure P zeolites show a similar trend (in the CEC dependence on temperature), P zeolite
Upon dehydration, water is lost from the pool of the being marginally superior throughout the tem- network to different extents. The loss of weight on perature range studied. heating increased with temperature. As the loss of 2. Zeolite P with 4A impurity has shown marginally weight at any particular temperature is known, the superior CEC values in the low temperature water still present in the sample at that temperature is domain (to even pure 4A and pure P). obtained by the difference. 3. CEC is dictated by the zeolitic water content.
4. Anhydrous zeolites have no building potential. 3.4. Exchange capacity 5. Powders dried at lower temperature have higher
CEC values. The water present in the original sample, and the
water still present after the drying step are known. The CEC is first arrived at experimentally as the number of mg of CaCO3 per g of zeolite. By dividing this CEC value by (100-% water content)/100, the CEC values t I on an anhydrous basis were obtained. These are pre- ~ a00 *c sented in Figs. 3 and 4 A closer examination of these
figures reveals: ~ U ~ f 700 %
PURE ZEOL I IE5
5O " ,
0 "Q O~ 0 " 0
. . . . . . . . . . . . ~ ~ ~oo TEMPERATUgE ( 'C )
i n . I
Fig. 3. Dependence of CEC on the drying temperature of pure ( l I t I 1 I zeolites ~ 3 ~ 300 *c
3SO IMPURE ZEOL ITE5
~ 2so j 200 *C
PURE 100 o c
r . . . . . . . . . . . . . ~b 3; 2b lo
T E MPE RA IURE I * C }
_2 O (CuK'~) Fig. 4. Dependence of CEC on the drying temperature of impure zeolites Fig. 5. XRD patterns of pure 4A heated to different temperatures.
58 P Sidheswaran, A.N. Bhat/Thermochimica Acta 298 (1997) 55-58
3.5. Mineralisation effect
The presence of the impurity phase influences the thermal behaviour of the pure component. This is well 800 c known in high temperature clay chemistry and this phenomenon is generally referred to as 'mineralisa- tion effect.' The XRD patterns of pure and mixed 4A and P samples were examined for establishing this 7o0 effect. Results Obtained with 4A are presented in 1 1 l / Figs. 5 and 6. Similar observations were made with ~ ~ ~ I I I ~ ] zeolite p. ~ ~ G00
It is evident from these figures that:
1. Mixed zeolites collapse at a lower temperature s00*c
than the pure sample. ~ 2. P has a tapotactic transition at around 350C and
gets converted into a different stable crystalline 4o0 c form of zeolite.
StructurecollapseandCEC ~ v ~ ~ ~ ~ 3oo*c 3.6.
1. In the case of pure zeolites, the crystallinity is ~ 1~l I , [ / retained even at higher temperatures. For instance, ~ ~ ~,~j~J~_ . , J 200 *c the crystallinity is > 90% even at 800C, whereas in the case of impure 4A, the crystallinity dropped J 1 , /
to about 90% at ,,~500C. Around 650C, the peak ~ A CONTAMINATE0 I I |/ lO0C
corresponding to 4A fingerprints in the lower 20 wtrH ~,~,_.A~ ]V~, J~ range (2-20), disappeared. ~b 3'0 20 i~ 2'
2. The crystallinity values of pure 4A samples treated ~ A ~.~o K., at 800 and 850C were 90 and ,-d0% respectively. The CES's of the above-treated samples were Fig. 6. XRD patterns of impure 4A (contaminated with P) heated
to different temperatures. ~25 mg/g of 4A. This finding indicates that the CEC reaches a minimum value prior to the collapse
References of the structure. 3. In the case of zeolite P, though a tapotactic
phase transition had occurred at ,,~350C, the  N.H. Ray, Inorganic Polymers, Academic Press (1978),128.  D.W. Breck, Zeolite Molecular Sieves: Structure, Chemistry
CEC values did not show any abrupt variation, and Use, John Wiley & Sons (1974). This seems to suggest that the cubic or tetragonal  A.I. Vogel, A Text Book of Quantitative Analysis, including types of zeolite P should not have any influence on Elementary Instrumental Methods of Analysis, ELBS and the CEC. Longman (1969), 436.